# adsorption and desorption kinetics of benzene derivatives ......

Post on 09-Feb-2018

215 views

Embed Size (px)

TRANSCRIPT

1

Supplementary material for the paper ADSO-D-12-00179 in Adsorption journal

(papers DOI : 10.1007/s10450-012-9462-7)

Adsorption and desorption kinetics of benzene derivatives on mesoporous

carbons

by Adam W. Marczewski*, Anna Derylo-Marczewska** and Agata Slota

*e-mail: Adam.Marczewski@umcs.lublin.pl , ** e-mail: annad@hektor.umcs.lublin.pl

*Dept. www: http://Radiochemistry.umcs.lublin.pl personal www: http://guide.adsorption.org

** Dept. www: http://SurfaceSci.umcs.lublin.pl

Contents

Appendix for the Theory - Flying start approach to solving kinetic equations ...............................1

Theory - supplementary figures .......................................................................................................3

Results and discussion - supplementary figures, tables and analyses..............................................3

Synthesis ......................................................................................................................................3

Isotherm data................................................................................................................................4

Kinetic data: .................................................................................................................................4

Preliminary kinetic analysis - Bangham plots..............................................................................7

Intraparticle diffusion model, IDM (Crank 1954). ......................................................................8

Pore diffusion model, PDM (Mc Kay 1996)..............................................................................11

gIKL/MOE plots ........................................................................................................................14

Fractal-like MOE plots...............................................................................................................19

Some comments on gIKL/MOE/SO fitting: ..............................................................................21

Appendix for the Theory - Flying start approach to solving kinetic

equations

If we know a solution (or some numerical procedure) of some kinetic equation at specific initial

conditions (cx,x) and the rate depends only on the temporary state of such system (e.g. for

Langmuir and SRT kinetics involving lateral interactions and energetic heterogeneity but not

intraparticle diffusion model) we may easily find more general solutions by using a simple general

geometric scheme called here the flying start approach. The initial conditions (co,o) of a given

adsorption system may be treated as a temporary state of some imaginary kinetics with the initial

conditions (cx,x) and the same equilibrium (ceq,eq). It means that in the coordinates of this

imaginary kinetics, (co,o) are flying start conditions of our real experiment and we should

extrapolate conditions backwards to (cx,x) (see Fig. 1 for adsorption scheme).

At our flying start, i.e. initial conditions of the real experiment (co,o), the adsorption progress of the

imaginary kinetics F is Fo and )1(' oo FFFF += . However, time of the real experiment t is

)(')'(')( oFtFtFt = where t (F ) is the time of the imaginary kinetics. For adsorption with x=0

2

(e.g. IKL) we have Fo=o/eq and )/()( oeqoeqeqox ccc = . For desorption with cx=0 (e.g.

dIKL) we obtain Fo=co/ceq and )/()( oeqeqooeqx cccc = . In general this technique may be used

for any kinetics with the rate which depends only on the temporary state of the system.

ceq

c(F)

c(F)

eq

eq

o-

o

o

(F)

(F)

0 00

0 1

1

co

F=Fo

F=F = /o o eq

F

F

cx

initial conditions extrapolated backwards to =0

initial conditions: and co o

equilibrium conditions: and ceq eq

c-c x

eq

backward-extrapolated

exp.

adsorption progress (backward-extrapolated start)

c-c o

eq

cx

co

(t)

ceq

equilibrium conditions: and ceq eq

initial conditions: and co o

real time

time from backward-extrapolated start

initial conditions backward-extrapolated to =0

c(t)

to0

0

Fig. S1. The idea and calculation scheme of the flying-start kinetic approach to adsorption kinetics with some pre-

adsorbed solute. Initial conditions: (co, o), equilibrium: (ceq, eq). F adsorption progress, F - adsorption progress of

the imaginary experiment with the same equilibrium (ceq, eq) and temporary (co, o) conditions.

ceq

c(F)=

cF

eq

x

o eq-

x eq- o

(F)=-F(

-)

x

xeq

0 00

0 1

1

co

c -ceq o

co

F=Fo

F=F =c /co o eq

F=F =(o - )/( - ) x o x eq

F

F

initial conditions extrapolated backwards to c=0

initial conditions: and co o

equilibrium conditions: and ceq eq

backward-extrapolated

exp.

desorption progress (backward-extrapolated start)

eq

(F)=-F(

-)

o

o

eq

c(F)=

c +F(

c-c

)

o

eqo

x

o

(t)eq

equilibrium conditions: and ceq eq

initial conditions: and co o

real time

time from backward-extrapolated start

initial conditions backward-extrapolated to =0c

c(t)

to0

0

Fig. S2. The idea and calculation scheme of the flying-start kinetic approach to desorption kinetics with non-zero

initial solute concentration. Initial conditions: (co, o), equilibrium: (ceq, eq). F desorption progress, F - desorption

progress of the imaginary experiment with the same equilibrium (ceq, eq) and temporary (co, o) conditions.

By using this method we may generalize simpler equations (e.g. IKL and dIKL to gIKL) with much

less effort than is required for analytical solution from scratch. Moreover, in the case of IKL and

dIKL the obtained equations are of the same type as the basic equations for standard initial

conditions (IKL for zero coverage, o =0 and dIKL for zero concentration, co=0). However, the

Langmuir batch equilibrium factor fL of such a kinetic fragment is always smaller in magnitude

|fL| than the value fx for the imaginary kinetics which it is part of, )1/()1( oxoxL FfFff = . The

only exceptions are the second order adsorption kinetics ( 1== xL ff ) and first order adsorption or

3

desorption kinetics ( 0== xL ff ) which do not change behavior if the initial conditions (o for

adsorption or co for desorption) are changed.

Theory - supplementary figures

0.0

0.5

1.0

0 1 2 3 = t/t 1/2

F

f L =1

f L = -1

ads

des 0

SOE

des

ads

SOE

0.0

0.2

0.4

0.6

0 0.5 1 = t/t 1/2

F

f L =1

f L = -1

0

des

ads

Fig. S3. Adsorption progress, F, vs. reduced time, =t/t1/2 for gIKL Eq. (6) (fL changes from -1 to 1 with 0.5 step). The

dashed lines correspond to the initial rates (right).

0.0

0.5

1.0

0 1 2 3ln(1 + )

F

f L =1f L = -1

ads

des0

SOE

des

ads

SOE

Fig. S4. Adsorption progress, F, vs. half-log reduced time scale, ln(1+), where =t/t1/2 for gIKL Eq. (6); fL changes

from -1 to 1 with 0.5 step.

Results and discussion - supplementary figures, tables and analyses

Synthesis

Synthesis and adsorption data were partly discussed in:

Derylo-Marczewska, A.; Marczewski, A.W.; Slota, A.: Kinetics of adsorption and desorption for selected organics from

aqueous solutions on mesoporous solids. Proc. 12th Polish-Ukrainian Symp. on Theoretical and Experimental Studies

4

of Interfacial Phenomena and Their Technological Applications (TESIP-12), ISBN 978-83-227-3180-2, Ameliwka

(Kielce), Poland, Aug 24-28, 2010, p.26 (only 1 page abstract).

Synthesis modification of the original methods (silica synthesis: Zhao et al. 1998; direct carbon synthesis: Kim et al. 2004) - see details below.

Carbon synthesis details:

Polymer1 (for W84,W87) Pluronic PE6400 (from BASF) - non-ionic copolymer (EO)13(PO)30(EO)13 , where EO-ethylene oxide, PO-propylene oxide (M = 2900 g/mol) Polymer2 (for W85) Pluronic PE9400 (from BASF) - non-ionic copolymer (EO)21(PO)47(EO)21 (M = 4600 g/mol) TEOS tetraethylorthosilicate, PhTEOS phenyl-triethylortosilicate TMB - 1,3,5-trimethylbenzene

1. Silicas: Dissolve 10 g of polymer in 360 ml of 1.6M HCl, add 10 g of TMB, stir slowly at 35C for 45 min, add 28 g TEOS and 6 g of PhTEOS, keep stirring for 20 hrs, put in autoclave at 70C- 120C for 24 hrs, cool down, put on fine filtrating paper and rinse with distilled water. Autoclave temperatures: 70C (for W84), 120C (W85), 100C (W87) were selected to obtain divergent silica and carbon properties

2. Carbonization: carbon-silica composite from as-synthesized silica (direct method): Add 4 g of water and 0.08 g of H2SO4 per 1 g of as-synthesized silica, mix for 30 min, put into vacuum dryer for 12 hrs at 100C, then keep at 160C for 12 hrs. Continue carbonization at 800C in nitrogen atmosphere for 6 hrs.

3. Etching: carbon from carbon-silica composite: KOH or NaOH in 50:50 EtOH/water solution

Typically only 2 g of carbon is obtained from the initial 10 g of polymer.

Isotherm data

Adsorption of SA is always much stronger than adsorption of BA and adso